Tensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density


 Janis Lyons
 2 years ago
 Views:
Transcription
1 Engineering Solid Mechanics 3 (2015) Contents lists available at GrowingScience Engineering Solid Mechanics homepage: Tensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density A. Campagnolo and F. Berto * University of Padova, Department of Management and Engineering, Stradella S. Nicola 3, Vicenza, Italy A R T I C L E I N F O A B S T R A C T Article history: Received September 6, 2014 Accepted 12 November 2014 Available online 12 December 2014 Keywords: Polymethylmethacrylate Unotch Vnotch Static Elasticity Strain energy In this paper, a volume criterion based on a simple scalar quantity, the mean value of the strain energy (SED), has been used to assess the static strength of notched components made of Polymethylmethacrylate (PMMA). The localstrainenergy based approach has been applied to a welldocumented set of experimental data recently reported in the literature. Data refer to blunt Unotched cylindrical specimens of commercial PMMA subjected to static loads and characterised by a large variability of notch tip radius (from 0.67 mm to 2.20 mm). Critical loads obtained experimentally have been compared with the theoretical ones, estimated by keeping constant the mean value of the strain energy in a welldefined small size volume. In addition, some new tests dealing with Vnotched specimens with end holes have been carried out to investigate the effect of the notch opening angle Growing Science Ltd. All rights reserved. 1. Introduction When we want to assess the strength of notched components, both under fatigue and static loads, there is the necessity of introducing a materialdependent parameter, which typically has units of length. In the literature there are different group of methodologies. The Cohesive Zone Model (CZM) is one of the most important approaches. It was first proposed for concrete and later successfully extended to brittle or quasibrittle failure of a large bulk of materials and in particular PMMA specimens (Gomez et al., 2000; Elices et al., 2002; Gomez et al., 2005). Another useful failure criteria, employed for analysing theoretically the brittle fracture in cracked or notched members, is the maximum tangential stress (MTS) approach (Ayatollahi et al., 2006, 2011; Ayatollahi and Aliha 2009; Torabi, 2013a, b,c; Mirsayar and Samaei, 2014). A coherent theory of fracture that can consistently account for the fracture behaviour of both sharp cracks and blunt notches was proposed by Sih (1974) by applying the strain energy density (SED) criterion to the bulk of the material near the notch surface. The parameter S is the product of the strain * Corresponding author. addresses: (F. Berto ) 2015 Growing Science Ltd. All rights reserved. doi: /j.esm
2 36 energy density and a small distance from the point of singularity. Failure was thought of as controlled by a critical value of S, whereas the direction of crack propagation is determined by imposing a minimum condition on S. Different from Sih's criterion, which is a pointwise criterion, the averaged strain energy density criterion (SED) states that brittle failure occurs when the mean value of the strain energy density over a control volume is equal to a critical energy (Lazzarin & Zambardi, 2001; Lazzarin & Berto, 2005; Berto & Barati, 2011; Lazzarin et al., 2014). For a review of the SED approach the reader can refer to some recent papers (Berto & Lazzarin, 2009; Lazzarin & Berto, 2014). An important advantage of the mean SED approach with respect to the stress based criteria is the mesh independency (Lazzarin et al., 2010). The latest developments and applications have been presented in (Pook et al., 2014; Campagnolo et al., 2015) by highlighting the capacity to automatically take into account also threedimensional effects. The approach will be applied here to a number of experimental data taken from the literature (Zheng et al., 2003) and obtained from static tests carried out on PMMA cylindrical specimens, weakened by blunt Unotches. The experimental values of the critical load are compared with the theoretical predictions based on SED showing a sound agreement. Finally to consider the effect of the notch opening angle some tests have been carried out by the present authors (Berto et al., 2013) on symmetric Vnotches with end holes. The final assessment based on SED shows a good agreement between experimental results and theoretical values. 2. Analytical Frame: strain energy density for blunt Vnotches under mode I loading The SED approach is based on the idea that under tensile stresses failure occurs when the averaged value of the strain energy over a control volume (area in plane models) W reaches the critical value W c, which obviously varies from material to material. If the material behaviour is ideally brittle, then W c can be evaluated by using simply the conventional ultimate tensile strength t, so that W c= t 2 /2E, where E is the modulus of elasticity. In the case of blunt notches, the area assumes a crescent shape, with R c being its maximum width as measured along the notch bisector line (Fig. 1c). By using the elastic maximum notch stress max, it is possible to determine the mean value of the SED (Lazzarin & Berto, 2005). Under plane strain conditions, a useful expression for Rc has been provided considering the crack case (Lazzarin & Zambardi, 2001; Lazzarin & Berto, 2005): R c 1 ν5 8ν 4π K σ IC t 2 r 0 R c (1) 2 2 R c R c R c +r 0 (a) (b) (c) Fig. 1. Critical volume definition for sharp Vnotch (a), crack (b) and blunt Vnotch (c). 3. Experimental data The SEDapproach is applied here to a set of data that refers to circumferentially Unotched roundrod specimens tested under tensile loading, made of a commercial unoriented PMMA (Zheng et al., 2003). The specimens were characterized by three values of the notch tip radius ρ = 0.67, 1.32 and 2.20 mm. The material was characterised by a Poisson s ratio = 0.4, a modulus of elasticity E = 3.20 GPa and a fracture toughness K IC 1.00 MPa m 0.5. The value of the linear elastic critical tensile stress at
3 A. Campagnolo and F. Berto / Engineering Solid Mechanics 2 (2015) 37 the notch root was MPa, while the critical strain energy W c was 0.90 MJ/m 3, respectively. The stressstrain curve showed a linear elastic trend up to failure. To consider also the effect of the notch opening angle some new tests have been carried out by the present authors on double symmetric Vnotched specimens with end holes characterized by a notch opening angle equal to 30 and 120. The geometry of the specimens is shown in Fig. 2. Three different notch root radii were used in the experiments: = 0.5, 1 and 2 mm. 10 mm 50 mm 2 10 mm 0.5, 1, 2 mm 200 mm Fig. 2. Geometry of the PMMA specimens weakened by Vnotches with end holes. Being the PMMA the same used in (Gomez et al., 2007), the critical stress has been confirmed equal to 130 MPa while the critical energy equal to W c= MJ/m 3. All tests were performed at room temperature under displacement control on a servocontrolled MTS biaxial testing device (100 kn/ 110 Nm, 75mm/ 55 ). The load was measured by a MTS cell with ± 0.5 % error at full scale. 4. Application of the SED approach Finite element (FE) modelling was performed using ANSYS 12.1 in order to determine the mean value of the strain energy density (SED) at failure relating to the different specimens. The simulations were conducted under purely linearelastic conditions, in a state of plane strain for the plain specimens while the axialsymmetry option was activated when considering the cylindrical specimens. The mesh was performed by using the eight nodes element (PLANE 82). By using Eq. 1 and the above mentioned properties for the material tested in (Zheng et al., 2003) and for the material tested by the present authors, Rc results to be mm in both cases. In order to evaluate the mean value of the strain energy density at failure, the critical loads obtained experimentally on the tested specimens have been directly applied to the FEmodels. 5. Results and discussion A synthesis in terms of the square root value of the local energy at failure, averaged over the control volume (of radius R c), obtained by FEanalysis and normalised with respect to the critical energy of the
4 38 material as a function of the notch tip radius is shown in Fig. 3 and 4 for the new data. The plotted parameter is proportional to the fracture load. All the values fall inside a scatter ranging from 0.8 to 1.2 and this states true for both the kind of PMMA considered in the present investigation. Then it is possible to consider the averaged strain energy density (SED) at failure as constant and equal to the critical value characteristic of the material. Fig. 3. Scatter of the strain energy density values at failure for circumferentially Unotched roundrod specimens made of PMMA (Zheng et al., 2003) Fig. 4. Scatter of the strain energy density values at failure for specimens weakened by symmetric V notches with end holes and made of PMMA In Fig. 5 the experimental values of the critical loads (open dots) have been compared with the theoretical assessed values based on the constancy of the SED in the control volume (solid lines). As shown in the figure it is evident that the trend of the predicted loads is in good agreement with the
5 A. Campagnolo and F. Berto / Engineering Solid Mechanics 2 (2015) 39 experimental one, being the maximum deviation less than 20% for the data taken from Zheng et al. (2003). Table 1 reports the results of the FEanalysis, in terms of averaged SED at failure, and the direct comparison between the mean experimental loads and the theoretical assessed values. Fig. 5. Critical load P cr versus notch radius, comparison between theoretical predictions and experimental data for specimens made of PMMA (Zheng et al., 2003); predictions based on 3 constant value W MJ / m c Table 1. Strain energy as obtained from numerical analyses of circumferentially Unotched roundrod specimens made of PMMA (Zheng et al., 2003). W c=0.903 MJ/m 3 D L a ρ P P th 1 mm mm mm mm N N MJ/m 3 W 0. 5 W / 1 W C Dealing with the new data, Fig. 6 shows the experimental values of the critical loads compared with the theoretical one, in the case of a notch opening angle equal to 30. The relative deviation between
6 40 experimental and theoretical values is always lower than 15%, in good agreement with previous tests under mode I loading (Lazzarin and Berto, 2005). Table 2 reports the results of the FEanalysis, in terms of averaged SED at failure, and the direct comparison between the mean experimental loads and the theoretical assessed values, for the new data. Fig. 6. Critical load P cr versus notch radius, comparison between theoretical predictions and experimental data for specimens weakened by symmetric Vnotches with end holes and 3 made of PMMA; predictions based on constant value Wc MJ / m ; 2α = 30 (a) 2α = 120 (b)
7 A. Campagnolo and F. Berto / Engineering Solid Mechanics 2 (2015) 41 Table 2. Strain energy as obtained from numerical analyses of specimens weakened by symmetric V notches with end holes and made of PMMA, W c= MJ/m 3 2α W B a ρ <P> P th 1 mm mm mm mm N N MJ/m 3 W 0. 5 W / 1 W C Conclusions An approach, useful for the assessment of the strength of notched components and based on the mean value of the strain energy over a small size area surrounding the tip of the notches, has been applied here to a number of experimental data taken from the literature and obtained from static tests carried out on PMMA cylindrical specimens, weakened by blunt Unotches. In addition some new data from PMMA Vnotched specimens with end holes are reported in the paper. The results of the synthesis based on SED show that the averaged values of the strain energy density at failure can be considered as a constant for the material and equal to the critical value, W c. The experimental loads can be assessed with a maximum error of ± 20% which in many cases remains in the range of ± 10%. References Ayatollahi, M. R., Aliha, M. R. M., & Hassani, M. M. (2006). Mixed mode brittle fracture in PMMA an experimental study using SCB specimens. Materials Science and Engineering: A, 417(1), Ayatollahi, M. R., & Aliha, M. R. M. (2009). Analysis of a new specimen for mixed mode fracture tests on brittle materials. Engineering Fracture Mechanics, 76(11), Ayatollahi, M. R., Aliha, M. R. M., & Saghafi, H. (2011). An improved semicircular bend specimen for investigating mixed mode brittle fracture. Engineering Fracture Mechanics, 78(1), Berto, F., & Lazzarin, P. (2009). A review of the volumebased strain energy density approach applied to Vnotches and welded structures. Theoretical and Applied Fracture Mechanics, 52(3), Berto, F., & Barati, E. (2011). Fracture assessment of Unotches under three point bending by means of local energy density. Materials & Design, 32(2), Berto, F., & Lazzarin, P. (2014). Recent developments in brittle and quasibrittle failure assessment of engineering materials by means of local approaches. Materials Science and Engineering: R: Reports, 75, Berto, F., Campagnolo, A., Elices, M., & Lazzarin, P. (2013). A synthesis of Polymethylmethacrylate data from Unotched specimens and Vnotches with end holes by means of local energy. Materials & Design, 49, Campagnolo, A., Berto, F., & Lazzarin, P. (2015). The effects of different boundary conditions on threedimensional cracked discs under antiplane loading. European Journal of MechanicsA/Solids., 50, Elices, M., Guinea, G. V., Gomez, J., & Planas, J. (2002). The cohesive zone model: advantages, limitations and challenges. Engineering fracture mechanics, 69(2),
8 42 Gómez, F. J., Elices, M., & Valiente, A. (2000). Cracking in PMMA containing U shaped notches. Fatigue & Fracture of Engineering Materials & Structures, 23(9), Gómez, F. J., Elices, M., & Planas, J. (2005). The cohesive crack concept: application to PMMA at 60 C. Engineering fracture mechanics, 72(8), Gómez, F. J., Elices, M., Berto, F., & Lazzarin, P. (2007). Local strain energy to assess the static failure of Unotches in plates under mixed mode loading. International Journal of Fracture, 145(1), Mirsayar, M., & Samaei, A. (2014). Application of maximum tangential stress criterion in determination of fracture initiation angles of silicon/glass anodic bonds. Engineering Solid Mechanics, 2(3), Lazzarin, P., & Zambardi, R. (2001). A finitevolumeenergy based approach to predict the static and fatigue behavior of components with sharp Vshaped notches. International Journal of Fracture, 112(3), Lazzarin, P., & Berto, F. (2005). Some expressions for the strain energy in a finite volume surrounding the root of blunt Vnotches. International Journal of Fracture, 135(14), Lazzarin, P., Berto, F., & Zappalorto, M. (2010). Rapid calculations of notch stress intensity factors based on averaged strain energy density from coarse meshes: theoretical bases and applications. International Journal of Fatigue,32(10), Lazzarin, P., Campagnolo, A., & Berto, F. (2014). A comparison among some recent energyand stressbased criteria for the fracture assessment of sharp Vnotched components under Mode I loading. Theoretical and Applied Fracture Mechanics. 71, Pook, L. P., Berto, F., Campagnolo, A., & Lazzarin, P. (2014). Coupled fracture mode of a cracked disc under antiplane loading. Engineering Fracture Mechanics, 128, Sih, G. C. (1974). Strainenergydensity factor applied to mixed mode crack problems. International Journal of fracture, 10(3), Torabi, A. (2013 a). Wide range brittle fracture curves for Unotched components based on UMTS model. Engineering Solid Mechanics, 1(2), Torabi, A. (2013 b). Failure curves for predicting brittle fracture in Vnotched structural components loaded under mixed tension/shear: An advanced engineering design package. Engineering Solid Mechanics, 1(3), Torabi, A. (2013 c). The equivalent material concept: application to failure of Onotches. Engineering Solid Mechanics, 1(4), Zheng, X. L., Wang, H., & Yan, J. H. (2003). Notch strength and notch sensitivity of polymethyl methacrylate glasses. Materials Science and Engineering: A, 349(1),
NOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationEstimation of the crack propagation direction in a mixedmode geometry via multiparameter fracture criteria
Focussed on characterization of crack tip fields Estimation of the crack propagation direction in a mixedmode geometry via multiparameter fracture criteria L. Malíková, V. Veselý Brno University of Technology,
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationVersion default Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 Responsable : François HAMON Clé : V6.03.161 Révision : 9783
Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 SSNP161 Biaxial tests of Summarized Kupfer: Kupfer [1] was interested to characterize the performances of the concrete under biaxial
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationTHERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE
THERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE L. DAHMANI, M.KOUANE Abstract In this paper are illustrated the principal aspects connected with the numerical evaluation of
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationDistinguishing strength from toughness. Understanding fracture toughness.
Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationMATERIALS SELECTION FOR SPECIFIC USE
MATERIALS SELECTION FOR SPECIFIC USE1 Subtopics 1 Density What determines density and stiffness? Material properties chart Design problems LOADING 2 STRENGTH AND STIFFNESS Stress is applied to a material
More informationAssessment of Fatigue Cracks in Rails
Procedia  Social and Behavioral Sciences 00 (2011) 000 000 Procedia Social and Behavioral Sciences www.elsevier.com/locate/procedia Conference Title (Transport Research Arena Europe 2012) Assessment of
More informationANALYTICAL AND EXPERIMENTAL EVALUATION OF SPRING BACK EFFECTS IN A TYPICAL COLD ROLLED SHEET
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 119130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationComposite structures are used extensively in aircraft, space vehicles, marine, and automotive
Finite Element Analyses of CompositetoSteel Adhesive Joints YuPing Yang George W. Ritter David R. Speth Edision Welding Institute Columbus, Ohio Finite element modeling can assist in the design of an
More informationFinite Element Analysis (FEA) Tutorial. Project 2: 2D Plate with a Hole Problem
Finite Element Analysis (FEA) Tutorial Project 2: 2D Plate with a Hole Problem Problem Analyze the following plate with hole using FEA tool ABAQUS P w d P Dimensions: t = 3 mm w = 50 mm d = mm L = 0 mm
More information2. FRACTURE MECHANICS
2. FRACTURE MECHANICS Igor Kokcharov 2.1 DEFECTS Structural materials have inner defects such as cracks, which are extreme stress concentrators. There are technological defects shown in diagrams A and
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationHW 10. = 3.3 GPa (483,000 psi)
HW 10 Problem 15.1 Elastic modulus and tensile strength of poly(methyl methacrylate) at room temperature [20 C (68 F)]. Compare these with the corresponding values in Table 15.1. Figure 15.3 is accurate;
More informationLap Fillet Weld Calculations and FEA Techniques
Lap Fillet Weld Calculations and FEA Techniques By: MS.ME Ahmad A. Abbas Sr. Analysis Engineer Ahmad.Abbas@AdvancedCAE.com www.advancedcae.com Sunday, July 11, 2010 Advanced CAE All contents Copyright
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationInvestigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter
Investigation of Stress Intensity Factor of Axial Compressor Blade of Helicopter Neelesh V K Mr. Manjunath M V Mr. Devaraj Dept. of Mechanical Engineering Asst prof, Dept. of Mechanical Engineering Asst
More informationMASTER DEGREE PROJECT
MASTER DEGREE PROJECT Finite Element Analysis of a Washing Machine Cylinder Thesis in Applied Mechanics one year Master Degree Program Performed : Spring term, 2010 Level Author Supervisor s Examiner :
More informationSTATIC AND DYNAMIC ANALYSIS OF CENTER CRACKED FINITE PLATE SUBJECTED TO UNIFORM TENSILE STRESS USING FINITE ELEMENT METHOD
INTERNATIONAL JOURNAL OF MECHANICAL ENGINEERING AND TECHNOLOGY (IJMET) International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 6340(Print), ISSN 0976 6340 (Print) ISSN 0976 6359
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationFEM analysis of the forming process of automotive suspension springs
FEM analysis of the forming process of automotive suspension springs Berti G. and Monti M. University of Padua, DTG, Stradella San Nicola 3, I36100 Vicenza (Italy) guido.berti@unipd.it, manuel.monti@unipd.it.
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More information3D WAVEGUIDE MODELING AND SIMULATION USING SBFEM
3D WAVEGUIDE MODELING AND SIMULATION USING SBFEM Fabian Krome, Hauke Gravenkamp BAM Federal Institute for Materials Research and Testing, Unter den Eichen 87, 12205 Berlin, Germany email: Fabian.Krome@BAM.de
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationRESIDUAL STRESS EFFECTS IN FRACTURE OF COMPOSITES AND ADHESIVES
RESIDUAL STRESS EFFECTS IN FRACTURE OF COMPOSITES AND ADHESIVES JOHN A. NAIRN ABSTRACT Because composites and adhesive joints are made from different phases with different thermal expansion coefficients,
More informationComputational Analysis of Stressstrain State, Dynamics, Strength and Stability of Loadbearing Concrete Structures of NPP Evaporative Cooling Towers
Prof. Alexandr Belostotskiy, Assoc. Prof. Sergey Dubinsky, PhD student Sergey Petryashev, PhD student Nicolay Petryashev Computational Analysis of Stressstrain State, Dynamics, Strength and Stability
More informationComparison of typical 3D printing materials [1]
Comparison of typical 3D printing materials [1] ABS Its strength, flexibility, machinability, and higher temperature resistance make it often a preferred plastic for engineers, and professional applications.
More informationTHE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE
THE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE Jaroslav Juracka, Vladimir Matejak Brno University of Technology, Institute of Aerospace Engineering juracka@fme.vutbr.cz;
More informationCRASH ANALYSIS OF AN IMPACT ATTENUATOR FOR RACING CAR IN SANDWICH MATERIAL
F2008SC016 CRASH ANALYSIS OF AN IMPACT ATTENUATOR FOR RACING CAR IN SANDWICH MATERIAL Boria, Simonetta *, Forasassi, Giuseppe Department of Mechanical, Nuclear and Production Engineering, University
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationFluid structure interaction of a vibrating circular plate in a bounded fluid volume: simulation and experiment
Fluid Structure Interaction VI 3 Fluid structure interaction of a vibrating circular plate in a bounded fluid volume: simulation and experiment J. Hengstler & J. Dual Department of Mechanical and Process
More informationThe Influence of Magnetic Forces on the Stability Behavior of Large Electrical Machines
The Influence of Magnetic Forces on the Stability Behavior of Large Electrical Machines Dr. H. Sprysl, Dr. H. Vögele, ABB Kraftwerke AG, CH5242 Birr Dr. G. Ebi, SENSOPLAN GmbH, D79801 Hohentengen a.h.
More informationCAD and Finite Element Analysis
CAD and Finite Element Analysis Most ME CAD applications require a FEA in one or more areas: Stress Analysis Thermal Analysis Structural Dynamics Computational Fluid Dynamics (CFD) Electromagnetics Analysis...
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN
ESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN Titulación: INGENIERO INDUSTRIAL Título del proyecto: MODELING CRACKS WITH ABAQUS Pablo Sanchis Gurpide Pamplona, 22 de Julio del
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationB. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS
B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions
More informationSTRESSSTRAIN RELATIONS
STRSSSTRAIN RLATIONS Strain Strain is related to change in dimensions and shape of a material. The most elementar definition of strain is when the deformation is along one ais: change in length strain
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationStress Analysis of an Aircraft Wing with a Landing Gear Opening Cutout of the Bottom Skin
Stress Analysis of an Aircraft Wing with a Landing Gear Opening Cutout of the Bottom Skin Kiran Shahapurkar 1, Ravindra Babu G 2 1 Lecturer, Department of Mechanical Engineering, Jain College of Engineering,
More informationFracture and strain rate behavior of airplane fuselage materials under blast loading
EPJ Web of Conferences 6, 6 42017 (2010) DOI:10.1051/epjconf/20100642017 Owned by the authors, published by EDP Sciences, 2010 Fracture and strain rate behavior of airplane fuselage materials under blast
More informationDUCTILE DAMAGE PARAMETERS IDENTIFICATION FOR NUCLEAR POWER PLANTS EXPERIMENTAL PART. Antonín PRANTL, Jan DŽUGAN, Pavel KONOPÍK
DUCTILE DAMAGE PARAMETERS IDENTIFICATION FOR NUCLEAR POWER PLANTS EXPERIMENTAL PART Antonín PRANTL, Jan DŽUGAN, Pavel KONOPÍK Škoda JS a.s., Pilsen, Czech Republic, EU, antonin.prantl@skodajs.cz COMTES
More informationBurst Pressure Prediction of Pressure Vessel using FEA
Burst Pressure Prediction of Pressure Vessel using FEA Nidhi Dwivedi, Research Scholar (G.E.C, Jabalpur, M.P), Veerendra Kumar Principal (G.E.C, Jabalpur, M.P) Abstract The main objective of this paper
More informationDEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS
1 th Canadian Masonry Symposium Vancouver, British Columbia, June 5, 013 DEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS Vladimir G. Haach 1, Graça Vasconcelos and Paulo
More informationSECTION 3 Progressive Ply Failure and Delamination Modeling
SECTION 3 Progressive Ply Failure and Delamination Modeling Composites Technology Day, January February 2012 S31 Composites Failure Modeling Look at types of problems you can solve today with MSC s composite
More information3. Test Methods for Evaluation of ESCR of Plastics
3. Test Methods for Evaluation of ESCR of Plastics A common laboratory request for ESCprone polymers is to check ESCR performance for quality control, competitive product evaluations, and research and
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationEXPERIMENTAL EVALUATION OF REINFORCED CONCRETE BEAM RETROFITTED WITH FERROCEMENT
Int. J. Struct. & Civil Engg. Res. 2013 Y V Ladi and P M Mohite, 2013 Research Paper EXPERIMENTAL EVALUATION OF REINFORCED CONCRETE BEAM RETROFITTED WITH FERROCEMENT Y V Ladi 1 * and P M Mohite 2 *Corresponding
More informationINVESTIGATION OF DEFORMATION BEHAVIOUR OF ALUMINIUM FOAM UNDER HIGHSTRAIN RATE LOADING AND COMPARISON WITH CONVENTIONAL ENERGY ABSORBING MATERIAL
INVESTIGATION OF DEFORMATION BEHAVIOUR OF ALUMINIUM FOAM UNDER HIGHSTRAIN RATE LOADING AND COMPARISON WITH CONVENTIONAL ENERGY ABSORBING MATERIAL P. Zlámal 1, T. Fíla 2, O. Jiroušek and V. Králík 4 Summary:
More informationCapturing complex nonlinear structural response through a series of linear analyses
Capturing complex nonlinear structural response through a series of linear analyses Supervisors: prof.dr.ir. Jan G. Rots dr.ir. Max A. N. Hendriks 1 BACKGROUND Reasons of research: Underground construction:
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON ENERGY DISSIPATION
EPJ Web of Conferences 6, 6 38009 (00) DOI:0.05/epjconf/000638009 Owned by the authors, published by EDP Sciences, 00 ANALYSIS OF THE FATIGUE STRENGTH UNDER TWO LOAD LEVELS OF A STAINLESS STEEL BASED ON
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationFATIGUE FRACTURE IN CONCRETE STRUCTURES
FATIGUE FRACTURE IN CONCRETE STRUCTURES Fabrizio Barpi and Silvio Valente Dipartimento di Ingegneria Strutturale e Geotecnica, Politecnico di Torino, Corso Duca degli Abruzzi 24, 10129 Torino. Email:
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationMesh Discretization Error and Criteria for Accuracy of Finite Element Solutions
Mesh Discretization Error and Criteria for Accuracy of Finite Element Solutions Chandresh Shah Cummins, Inc. Abstract Any finite element analysis performed by an engineer is subject to several types of
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationExercise 1: Three Point Bending Using ANSYS Workbench
Exercise 1: Three Point Bending Using ANSYS Workbench Contents Goals... 1 Beam under 3Pt Bending... 2 Taking advantage of symmetries... 3 Starting and Configuring ANSYS Workbench... 4 A. PreProcessing:
More informationEvaluating the Elastic Modulus of Lightweight Aggregate
Evaluating the Elastic Modulus of Lightweight Aggregate HowJi Chen, Tsong Yen, and KuanHung Chen HowJi Chen is an associate professor of Civil Engineering at National Chung Hsing University in Taiwan.
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More informationShort and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1
Short and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1 Mr. R. K. Nalla, Dr. J. P. Campbell and Professor R. O. Ritchie 2 Department of Materials Science and Engineering University
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationUnit 48: Structural Behaviour and Detailing for Construction. Chapter 13. Reinforced Concrete Beams
Chapter 13 Reinforced Concrete Beams Concrete is a material strong in its resistance to compression, but very weak indeed in tension. good concrete will safely take a stress upwards of 7 N/mm 2 in compression,
More informationINJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS
INJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS Tom Kimerling University of Massachusetts, Amherst MIE 605 Finite Element Analysis Spring 2002 ABSTRACT A FEA transient thermal structural
More informationStress and deformation of offshore piles under structural and wave loading
Stress and deformation of offshore piles under structural and wave loading J. A. Eicher, H. Guan, and D. S. Jeng # School of Engineering, Griffith University, Gold Coast Campus, PMB 50 Gold Coast Mail
More informationDESIGN AND ANALYSIS OF BRIDGE WITH TWO ENDS FIXED ON VERTICAL WALL USING FINITE ELEMENT ANALYSIS
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 3444, Article ID: IJCIET_07_02_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationThe Mechanical Properties of Glass
The Mechanical Properties of Glass Theoretical strength, practical strength, fatigue, flaws, toughness, chemical processes Glass Engineering 150:312 Professor Richard Lehman Department of Ceramics and
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationComputer Aided Engineering (CAE) Techniques Applied To Hip Implant
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 3 Computer Aided Engineering (CAE) Techniques Applied To Hip Implant 1, M. S. Abo_Elkhair, 2, M. E. AboElnor,
More informationANALYSIS FOR BEHAVIOR AND ULTIMATE STRENGTH OF CONCRETE CORBELS WITH HYBRID REINFORCEMENT
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 10, Oct 2015, pp. 2535 Article ID: IJCIET_06_10_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=10
More informationScienceDirect. The Numerical Analysis of the Joint of the Steel Beam to the Timber Girder
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 91 (2014 ) 160 164 XXIII RSP seminar, Theoretical Foundation of Civil Engineering (23RSP) (TFoCE 2014) The Numerical Analysis
More informationANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS
Nordic Steel Construction Conference 212 Hotel Bristol, Oslo, Norway 57 September 212 ANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS Marouene Limam a, Christine Heistermann a and
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationStress Relaxation Study of Paper and Plastic Film based Packaging Material
Master's Degree Thesis ISRN: BTHAMTEX2009/D02SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More informationExperimental research on joint behavior of H2section beams with flanges and end2plates connected by non2completely penetrated welds
26 3 Vol. 26 No. 3 2005 6 Journal of Building Structures June 2005 : 10006869(2005) 030070  08 H 1 1 2 3 4 (11 200092 ; 21 ( ) 201613 ; 31 201103 ; 41 310003) : H 24 6 : ; H : ; ; ; ; : TU39215 TU31711
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationUltrasonic Technique and Device for Residual Stress Measurement
Ultrasonic Technique and Device for Residual Stress Measurement Y. Kudryavtsev, J. Kleiman Integrity Testing Laboratory Inc. 80 Esna Park Drive, Units 79, Markham, Ontario, L3R 2R7 Canada ykudryavtsev@itlinc.com
More informationEUROLAB 25 years. The role of metrology and testing to characterize materials and products. EUROLAB 25th Anniversary Seminar
EUROLAB 25 years The role of metrology and testing to characterize materials and products April 9, 2015, Odense Danmark 1 Origin of Conformity Assessment The New Approach for the European Economic Community
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationNonLinear Materials. Introduction. Preprocessing: Defining the Problem
NonLinear Materials Introduction This tutorial was completed using ANSYS 7.0 The purpose of the tutorial is to describe how to include material nonlinearities in an ANSYS model. For instance, the case
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More informationThe Rock Cutting Process of Road Headers Laboratory Tests and Numerical Simulation
The Rock Cutting Process of Road Headers Laboratory Tests and Numerical Simulation Antretter, Galler, Pittino  Montanuniversitaet Leoben, Austria Gimpel, Kargl  Sandvik Mining and Construction GmbH,
More information